Active Standard ASTM C1611 / C1611M | Developed by Subcommittee: C09.47
Book of Standards Volume: 04.02
Historical (view previous versions of standard)
Significance and Use
This test method provides a procedure to determine the slump flow of self-consolidating concrete in the laboratory or the field.
This test method is used to monitor the consistency of fresh, unhardened self-consolidating concrete and its unconfined flow potential.
It is difficult to produce self-consolidating concrete that is both flowable and nonsegregating using coarse aggregates larger than 25 mm [1 in.]. Therefore, this test method is considered applicable to self-consolidating concrete having coarse aggregate up to 25 mm [1 in.] in size. Appendix X1 provides non-mandatory visual rating criteria that may be used to classify the ability of a self-consolidating concrete mixture to resist segregation (stability).
The rate at which the concrete spreads is related to its viscosity. Appendix X1 provides a non-mandatory procedure that may be used to provide an indication of relative viscosity of self-consolidating concrete mixtures.
1.1 This test method covers the determination of slump flow of self-consolidating concrete.
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.3 The text of this standard references notes and footnotes that provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of the standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (WARNING
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C125 Terminology Relating to Concrete and Concrete Aggregates
C143/C143M Test Method for Slump of Hydraulic-Cement Concrete
C172 Practice for Sampling Freshly Mixed Concrete
C173/C173M Test Method for Air Content of Freshly Mixed Concrete by the Volumetric Method
C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials
ICS Number Code 91.100.30 (Concrete and concrete products)